Research Article  Open Access
Failure Assessment for the HighStrength Pipelines with ConstantDepth Circumferential Surface Cracks
Abstract
In the oil and gas transportation system over long distance, application of highstrength pipeline steels can efficiently reduce construction and operation cost by increasing operational pressure and reducing the pipe wall thickness. Failure assessment is an important issue in the design, construction, and maintenance of the pipelines. The small circumferential surface cracks with constant depth in the welded pipelines are of practical interest. This work provides an engineering estimation procedure based upon the GE/EPRI method to determine the Jintegral for the thinwalled pipelines with small constantdepth circumferential surface cracks subject to tension and bending loads. The values of elastic influence functions for stress intensity factor and plastic influence functions for fully plastic Jintegral estimation are derived in tabulated forms through a series of threedimensional finite element calculations for different crack geometries and material properties. To check confidence of the Jestimation solution in practical application, Jintegral values obtained from detailed finite element (FE) analyses are compared with those estimated from the new influence functions. Excellent agreement of FE results with the proposed Jestimation solutions for both tension and bending loads indicates that the new solutions can be applied for accurate structural integrity assessment of highstrength pipelines with constantdepth circumferential surface cracks.
1. Introduction
The growing demand for energy and natural resources has been pushing exploration and production activities of oil and natural gas. In particular, application of thinwalled highstrength steel has become a trend in the oil and gas transportation system over long distance, which can improve the transportation efficiency by highpressure operation and reduce the pipe laying cost by reducing the wall thickness of pipes [1, 2]. Research projects have then been focused on the development of API grades X80 and X100 and more recently to grade X120 [1]. The highgrade pipeline steels have high yieldtoultimate tensile strength ratio, which means they have relatively low strainhardening ability. For the highstrength pipelines adopted in industries, the mean diametertothickness ratio D/t generally ranges from 50 to 100, such as the grade API 5L X80 steel applied on TransCanada system.
The longdistance oil and gas pipes are joined by girth weld. Common failures in pipelines result primarily from the weld defects. The failure assessment of cracklike flaws is an important issue in design and maintenance of the pipeline systems. Specifically, the fracture parameter Jintegral has been widely used in the structural integrity assessment of defective pipes. Full threedimensional finite element (FE) analyses can provide accurate results for the fracture response. However, FE analyses require large computational time, expertise, and resources, which make the numerical computation quite expensive to be used routinely; hence, they are not suitable for engineering structural integrity assessment. Therefore, the simplified Jestimation scheme with much less computational cost is highly desired from the view of engineering application.
Based upon the fully plastic Jintegral solution developed by Shih and Hutchinson [3], Kumar et al. [4] introduced the widely known GE/EPRI Jestimation approach for twodimensional geometries. Afterwards, the original work was extended by various researchers [5–14] to include additional geometries and loading conditions. Another popular Jestimation method is the reference stress approach which adopts the plastic limit load as the reference stress [15]. Based upon the FE results for pipes with varying geometries under different loading conditions, it was proposed that the reference stress could be redefined by an “optimized reference load” (rather than the plastic limit load) [16–19]. This method is termed as an enhanced reference stress method and can improve the accuracy in J estimation. However, it should be noted that these works mainly cover the cases of cracked pipes having mean diametertothickness ratio (D/t) not more than 40, while the values of D/t for highstrength pipelines are normally larger than 50.
To verify the applicability limit of the existing GE/EPRI method with regard to the diametertothickness ratio D/t, Cho et al. [20] have explored the Jestimation schemes for semielliptical surfacecracked pipes with D/t ranging from 10 to 120. Park et al. [21] have performed several FE analyses for pipes with a short circumferential throughwall crack. As pointed by those previous works [20–22], an application of existing solutions would result in inaccurate structural integrity assessment results when thinwalled pipes with large diameter are considered. If existing GE/EPRI solution, whose applicability is D/t ≤ 40, is directly extrapolated to thinwalled pipes with D/t > 60, the Jintegral would be nonconservative compared with the FE results [20, 21]. Underestimation of the crackdriving force might be very dangerous in the engineering failure assessment, which needs to be avoided. Therefore, extension of the estimation methods is urgently required for thinwalled pipes. Furthermore, in most of previous works, the surface cracks are usually modeled as elliptical configuration. The surface cracks with constant depth might represent well the weld defects commonly observed in pipelines [23]. Moreover, based upon the limits routinely adopted in design as well as nondestructive testing examination, such as API 1104 [24], small cracks are often a major concern for the welded pipes with large diameter. In this content, Jestimation solutions for thinwalled pipes with small constantdepth cracks need to be developed to overcome the limitations of the existing solutions.
This paper focuses on extending Jestimation solutions for highstrength pipelines with small constantdepth cracks. A series of elastic and elasticplastic FE analyses for the thinwalled pipes with D/t ranging from 50 to 100 under tension and bending loads are conducted in this paper. The analyses involve small constantdepth cracks with crack depthtothickness ratio a/t ranging 0.1–0.4 and normalized crack length θ/π ranging 0.01–0.08 for pipes with different strainhardening properties. By analyzing the FE results, the values of elastic influence functions for elastic stress intensity factor K and plastic influence functions for fully plastic Jintegral are proposed in tabulated forms based upon GE/EPRI estimation method. To show the efficiency of the estimation method for idealized Ramberg–Osgood material, Jintegral values obtained from the new elastic and plastic influence functions are compared with those from detailed threedimensional FE analyses. Moreover, to check confidence of the Jestimation solution in practical application, elasticplastic FE analyses are also conducted using experimental stressstrain data for three typical grade pipeline steels.
2. The GE/EPRI Method for Estimation
2.1. The EPRI Methodology
To estimate elasticplastic Jvalues for a cracked body, the GE/EPRI engineering method [3, 4] was developed based on FE solutions using deformation plasticity theory. The method assumes that the constitutive law for the materials can be characterized by the Ramberg–Osgood model:where σ is the true stress, ε is the true strain, σ_{0} is the yield stress, E is the elastic modulus, ε_{0} = σ_{0}/E is the corresponding reference strain, α is a dimensionless constant, and n defines the strainhardening exponent.
The GE/EPRI estimation method evolved from the two limiting cases of elastic and fully plastic conditions. The elasticplastic Jintegral is split into elastic and plastic components aswhere the subscript “e” denotes the elastic part of J, adjusted by a plastic zone correction using the effective crack length a_{e}, and “p” refers to plastic contributions. The elastic component J_{e} can be expressed via the stress intensity factor K bywhere = E for plane stress condition and = E/(1 − ν^{2}) for plane strain condition, with ν representing the Poisson ratio. Irwin [25] proposed that the plastic zone corrected crack length a_{e} can be obtained bywhere a is the crack length, β = 2 for plane stress, and β = 6 for plane strain conditions.
In 1976, Shih and Hutchinson [3] developed a new method for fully plastic Jintegral solutions. Upon consideration of a fully plastic cracked structure in which the elastic strains ε_{e} are vanishingly small compared with the plastic strains ε_{p}, the material defined by (1) follows a pure powerlaw stressstrain curve:
Under such assumption and close to the crack tip, the crack tip stress fields are given by the HRR singularity [26]where (r, φ) are polar coordinates centered at the crack tip, I_{n} is an integration constant, and are dimensionless stress functions. The HRR equation can be rewritten in the form of Jintegral:
With the application of Ilyushin’s theorem [27] that the fully plastic stresses are simply proportional to the applied load P, the fully plastic J given by (7) can be expressed in terms of the applied load aswhere W is the component width, b = W − a defines the uncracked ligament, represents additional characteristic length for the component, and h_{1} is the plastic influence function dependent on crack size, specimen geometry, and strainhardening exponent. In (8), the generalized load is normalized by a reference load P_{ref} which may be freely chosen provided it is proportional to σ_{0} but is often identified with the plastic limit load of the cracked component P_{L}.
2.2. Extension to Circumferentially Cracked Pipes
Figure 1 shows the relevant pipe and crack dimensions for circumferentially cracked pipes subjected to tensile load T and bending moment M. The circumferential surface crack in this work is assumed to be of constant depth a and length 2c with an end radius equal to the crack depth (as displayed in Figure 1). For the thinwalled pipes with large diameter, the circumferential crack angle 2θ is related to the crack length by
(a)
(b)
For circumferential surface cracks, the stress intensity factor can be expressed aswhere F is the elastic influence function and σ denotes the applied stress due to axial loading or bending moment by the following equation:where t is the pipe wall thickness, R denotes the mean radius (R = D/2), and R_{o} and R_{i} are the external and internal radii, respectively. Once the elastic influence function F is determined, the elastic term of J, J_{e}, can be calculated using (3). Then, the effective crack depth is obtained by (4). Noting that pipes with circumferential partthrough defects can be in between plane stress and plane strain conditions, the plane strain constant of 6 in (4) is valid only when the plasticity is confined within a dominantly elastically behaving body [16, 17]. On the other hand, if the plasticity effect is much more significant even below the widespread plasticity level, the plane stress constant of 2 is retained [17]. By FE analyses for the small circumferential partthrough defects, an empirical value of constant parameter β is adopted in this work (β = 2 for pipes with n = 10 and β = 3 for pipes with n ≥ 15).
To obtain the fully plastic part of the Jintegral for the circumferentially cracked pipes, (8) can be rewritten aswhere the uncracked ligament is b = t − a and the generalized load P_{L} is either the limit tensile load T_{L} or the plastic limit moment M_{L}, given by [28]. The tensile load T_{L} and the plastic limit moment M_{L} are expressed as
3. Finite Element Analysis
A series of parametric finite element simulations of circumferentially cracked pipes subjected to tensile load and bending moment have been conducted. The thinwalled pipes with large diameter are of main concern; here, two typical mean diametertothickness ratios are considered, namely, D/t = 50 and 100. Pipe wall thickness t is fixed to be 20 mm in the present work. As the weld pass height governs the flaw sizes in girthwelded pipelines, which is typically 2–6 mm in height [29], the values of crack depthtothickness ratio a/t are rationally selected as a/t = 0.1, 0.2, 0.3, and 0.4 in this work. Small cracks (2c ≤ 250 mm) are of practical interest in girthwelded pipelines [30]; therefore, the normalized crack lengths have been chosen as θ/π = 0.01 and 0.08 for pipes with D/t = 50 and θ/π = 0.01 and 0.04 for pipes with D/t = 100. To make the end effects on the computed fracture parameter Jintegral negligible, the total length of a pipe segment 2L is assumed to be six times the outer diameter [23].
In this paper, all analyses were performed by the commercial FE program, ABAQUS. Figure 2 shows a typical finite element mesh for the thinwalled pipe with a/t = 0.2, θ/π = 0.01, and D/t = 100. Similar meshes were employed for models with other crack depths and crack lengths. Considering the symmetry conditions, only onequarter of the pipe was modeled to improve the computational efficiency as shown in Figure 2. Symmetry boundary conditions were prescribed on the two surfaces whose normal direction is zaxis (z = 0 in Figure 1(a)) as well as on the midsection of the pipe (x = 0 in Figure 1(a), except the crack face). A reference point is defined at the uncracked end of the model and tied to all nodes at that end via the MPC (multipoint constraint). Tension is applied by specifying axial displacement to the reference node, and bending is applied by imposing a rotation to the reference point. The applied load is determined from the force acting on the reference point.
Elastic and elasticplastic FE analyses were performed to calculate the elastic fracture parameter K and the elasticplastic fracture parameter Jintegral at the deepest point of the surface cracks. For elastic analyses, an isotropic material was assumed with Young’ modulus E = 200 GPa and Poisson’ ratio ν = 0.3. For elasticplastic analyses, the material was assumed to follow the Ramberg–Osgood relation described by (1). In the parametric analyses, yield stress and dimensionless constant are fixed to σ_{0} = 400 MPa and α = 1. The hardening exponent of n = 10 corresponds to pipeline steels of grade API 5L X60 to X65, and n = 20 represents API 5L X80 or above [14, 31]. Therefore, three different values of the strainhardening index n are chosen, that is, n = 10, 15, and 20.
The values of Jintegral are calculated from the FE results using a domain integral method, as a function of applied load. Noting that the overall deviation of the Jintegral values, respectively, calculated from ten contours was less than a few percent, the confidence of the FE results was gained by the path independence of the Jintegral values. Thus, the Jintegral values were calculated from the mean of second to tenth contours after excluding the one immediately surrounding the crack tip. For elastic analyses, the calculated Jintegral values were converted to elastic fracture parameters K by (3).
To make further confidence in the accuracy of the numerical results, elastic and plastic FE results were compared with existing solution. For constantdepth surface cracks, the applicability of Zahoor’s solution [5] is 10 ≤ D/t ≤ 20 and 0.05 ≤ θ/π ≤ 1. Figure 3 shows comparisons of F values obtained from the FE analyses and Zahoor’s solution [5] for pipes with a/t = 0.4 and θ/π = 0.08. Figure 4 compares the numerical Jintegral values by detailed FE analysis with Zahoor’s solution [5]. As shown in Figure 3, the difference between the values of the elastic influence function F from FE analyses and those from Zahoor [5] is minor when D/t is around 20. The Jintegral values from FE and Zahoor’s solution [5] are found to be consistent with each other for the relatively thickwalled pipe with D/t = 20 as displayed in Figure 4. Therefore, the FE analyses are sufficiently validated for this study. On the other hand, it can be seen from Figure 3 that the deviation of the elastic influence function F by FE analyses from those of Zahoor [5] increases with the growth of D/t for pipes with D/t > 20, which means a new elastic influence function needs to be proposed for the application to the thinwalled pipes. To check the applicability of the existing GE/EPRI method with regard to D/t, elasticplastic FE analysis is also carried out for thinwalled pipes with D/t = 50. Figure 5 shows comparisons of Jintegral versus applied load obtained from the FE analyses and Zahoor’s solution [20] for thinwalled pipes with D/t = 50. As shown in Figure 5, the existing GE/EPRI solution underestimates the Jintegral when thinwalled pipes with small cracks are considered. Therefore, an extension of existing GE/EPRI method is conducted in the following section for the thinwalled pipes with small cracks.
(a)
(b)
4. Results and Discussion
4.1. New Elastic Influence Function and Plastic Influence Function
By performing the elastic FE analyses for the thinwalled pipes with D/t = 50 and 100, the values of F for the stress intensity factor under tension are given in Table 1. Results of F for these pipes under bending are tabulated in Table 2.


For circumferentially cracked pipes, new plastic influence function h_{1} is calculated using the equation for fully plastic part of the Jintegral in (12), which is rewritten as
Note that the calculated values of h_{1} depend on the load magnitude, as shown in Figure 6. As h_{1} represents a fully plastic condition, the values of h_{1} in (14) are taken at sufficiently high load level in which plastic strains dominate elastic strains. Table 3 lists the values of the plastic function h_{1} for the circumferentially cracked pipes with varying material properties under tension. Results of h_{1} for the pipes under bending are tabulated in Table 4.
(a)
(b)


An illustrative validation of the GE/EPRI procedure for Jintegral estimation of the idealized Ramberg–Osgood material is presented here. By using the GE/EPRI method with newly proposed elastic and plastic influence functions, the values of elasticplastic Jintegral are estimated and compared with those from FE results. Figure 7 refers to the pipes under tension having D/t = 100, a/t = 0.2, and θ/π = 0.01. Figure 8 shows the results for the pipes with the same configuration under bending. In Figures 7 and 8, new GE/EPRI means the GE/EPRI method with newly generated elastic and plastic influence functions. As shown in these two figures, the results of GE/EPRI estimation method with new elastic and plastic influence functions agree well with the FE results. Therefore, by deriving the effective values of influence functions, Jestimation procedure based upon the GE/EPRI method can be applied to the highstrength pipelines with small constantdepth cracks, which is of practical interest.
(a)
(b)
(c)
(a)
(b)
(c)
4.2. Application for Pipeline Steels
To show the effectiveness of proposed Jintegral estimation solutions, additional elasticplastic threedimensional FE analyses are performed. The FE procedures are similar to those in Section 3, except material properties. For validation in the pipeline industries, experimental true stressstrain data for the three different materials API 5L X70, X80, and X90 at the room temperature are considered, instead of idealized Ramberg–Osgood materials. Figure 9 shows the experimental true stressstrain data by uniaxial tension for the three materials. The entire true stressstrain data up to the ultimate tensile strength are fitted to determine the Ramberg–Osgood constants in (1). The best combination of α and n can be firstly obtained by leastsquares fit to the experimental data for one pipeline. It is found that n approaches 10 for X70 steel and 15 for X80 and X90 steels. Then, the values of n are fixed to 10 for X70 steel and 15 for X80 and X90 steels; the corresponding values of α are obtained by leastsquares fit method. The resulting Ramberg–Osgood fitting parameters are listed in Table 5, and the fitted Ramberg–Osgood curves are rather satisfactory as shown in Figure 9.

For a given material, the experimental true stressplastic strain data are directly adopted in the FE analysis and thinwalled pipes with D/t = 100, a/t = 0.2, and θ/π = 0.04. FE results are extracted by the method described in Section 3. The material parameters listed in Table 5 and values of F and h_{1} given in Section 4.1 are used to estimate the Jintegral. Figure 10 compares the estimated Jintegral with FE results for pipes under tension. Figure 11 provides similar results for pipes under bending. Excellent agreement shows that the newly proposed elastic and plastic influence functions can be successfully used to predict Jintegrals in pipeline industries.
(a)
(b)
(c)
(a)
(b)
(c)
5. Conclusions
Applicability of Jestimation solutions based upon GE/EPRI approach was extended to thinwall highstrength pipelines with small circumferential surface cracks, subject to tension and bending loads. Attention is directed to thinwalled highstrength steels in the oil and gas transportation system, which have relatively high strainhardening exponent. Size of the small cracks with constant depth considered in this work covers the range of practical interest in the welded pipelines.
Threedimensional FE analyses are conducted for the circumferentially cracked pipes with different crack geometries and material properties. By FE analyses for idealized Ramberg–Osgood materials, values of the new elastic influence function F for stress intensity factor and the new plastic influence function h_{1} for fully plastic J solutions are tabulated as a function of crack depthtothickness ratio a/t, normalized crack length θ/π, and mean diametertothickness ration D/t. The proposed Jestimation solutions are validated against threedimensional FE analyses by using experimental stressstrain data for three typical pipeline steels. Based on the excellent agreement between the Jestimation solution and the FE analyses, it is found that the proposed Jestimation solutions can be successfully used to predict the Jintegral for the highstrength pipelines with small circumferential surface cracks under tension and bending loads.
Nomenclature
a:  Crack depth 
a_{e}:  Effective crack length 
b:  Uncracked ligament 
c:  Halflength for a crack 
D:  Mean diameter of a pipe 
E:  Young’s modulus 
E^{′}:  “Effective” Young’s modulus 
F:  Elastic influence function for elastic stress intensity factor 
:  Plastic influence function for J_{p} in the GE/EPRI method 
I_{n}:  Integration constant for HRR fields 
J:  Jintegral 
J_{e}:  Elastic component of Jintegral 
J_{p}:  Plastic component of Jintegral 
K:  Elastic stress intensity factor 
L:  Halflength of a pipe 
M:  Bending moment 
M_{L}:  Plastic limit bending moment 
n:  Strainhardening exponent 
P:  Generalized load 
P_{L}:  Plastic limit load of a cracked pipe 
:  Reference load of a cracked pipe 
r, φ:  Polar coordinates 
R:  Mean radius of a pipe 
R_{i}:  Internal radius of a pipe 
R_{o}:  External radius of a pipe 
t:  Pipe wall thickness 
T:  Tensile load 
T_{L}:  Plastic limit tensile load 
x, y, z:  Rectangular coordinates 
α:  Dimensionless constant for Ramberg–Osgood material 
β:  Constant parameter (β = 2 for plane stress and β = 6 for plane strain) 
ε:  Strain 
:  Reference strain (ε_{0} = σ_{0}/E) 
ε_{p}:  Plastic strain 
θ:  Onehalf of a circumferential crack angle 
:  Characteristic length 
ν:  Poisson's ratio 
σ:  Stress 
:  Yield stress 
σ_{ij}:  Stress components 
:  Dimensionless stress functions for HRR fields. 
Conflicts of Interest
The authors declare that there are no conflicts of interest regarding the publication of this paper.
Acknowledgments
This work was supported by the National Key Research and Development Program of China (no. 2017YFB0702003), the Nature Science Foundation of China (Grant nos. 11132011, 11472287, and 11572324), the Key Research Program of Frontier Sciences (Grant no. QYZDJSSWJSC011), the Strategic Priority Research Program of the Chinese Academy of Sciences (Grant nos. XDB22040302 and XDB22040303), and the CASSAFEA International Partnership Program for Creative Research Teams.
References
 B. Tanguy, T. T. Luu, G. Perrin, A. Pineau, and J. Besson, “Plastic and damage behaviour of a high strength X100 pipeline steel: experiments and modelling,” International Journal of Pressure Vessels and Piping, vol. 85, no. 5, pp. 322–335, 2008. View at: Publisher Site  Google Scholar
 Y. Terada, H. Tamehiro, H. Morimoto et al., “X100 linepipe with excellent HAZ toughness and deformability,” ASME Conference Proceedings, vol. 2003, no. 36835, pp. 287–294, 2003. View at: Google Scholar
 C. F. Shih and J. W. Hutchinson, “Fully plastic solutions and largescale yielding estimates for plane stress crack problems,” Journal of Engineering Materials and Technology, vol. 98, no. 4, pp. 289–295, 1976. View at: Publisher Site  Google Scholar
 V. Kumar, M. D. German, and C. F. Shih, “An engineering approach for elasticplastic fracture analysis,” Electric Power Research Institute, Palo Alto, CA, USA, 1981, EPRI Report NP1931. View at: Google Scholar
 A. Zahoor, “Ductile fracture handbook,” Electric Power Research Institute, Palo Alto, CA, USA, 1989, EPRI Report NP6301D. View at: Google Scholar
 M. S. G. Chiodo and C. Ruggieri, “J and CTOD estimation procedure for circumferential surface cracks in pipes under bending,” Engineering Fracture Mechanics, vol. 77, no. 3, pp. 415–436, 2010. View at: Publisher Site  Google Scholar
 J. Foxen and S. Rahman, “Elasticplastic analysis of small cracks in tubes under internal pressure and bending,” Nuclear Engineering and Design, vol. 197, no. 12, pp. 75–87, 2000. View at: Publisher Site  Google Scholar
 V. Kumar, M. D. German, W. W. Wilkening, W. R. Andrews, H. G. Delorenzi, and D. F. Mowbray, “Advances in elastic–plastic fracture analysis,” Electric Power Research Institute, Palo Alto, CA, USA, 1984, EPRI Report NP3607. View at: Google Scholar
 V. Kumar and M. D. German, “Elasticplastic fracture analysis of throughwall and surface flaws in cylinders,” Electric Power Research Institute, Palo Alto, CA, USA, 1988, EPRI Report NP5596. View at: Google Scholar
 M. Paredes and C. Ruggieri, “Engineering approach for circumferential flaws in girth weld pipes subjected to bending load,” International Journal of Pressure Vessels and Piping, vol. 125, pp. 49–65, 2015. View at: Publisher Site  Google Scholar
 R. Mohan, A. Krishna, F. W. Brust, and G. M. Wilkowski, “Jestimation schemes for internal circumferential and axial surface cracks in pipe elbows,” Journal of Pressure Vessel Technology, vol. 120, no. 4, pp. 418–423, 1998. View at: Publisher Site  Google Scholar
 J. Chattopadhyay, A. K. S. Tomar, B. K. Dutta, and H. S. Kushwaha, “Elasticplastic J and COD estimation schemes for throughwall circumferentially cracked elbow under inplane closing moment,” Engineering Fracture Mechanics, vol. 72, no. 14, pp. 2186–2217, 2005. View at: Publisher Site  Google Scholar
 J. Chattopadhyay, “Improved J and COD estimation by GE/EPRI method in elastic to fully plastic transition zone,” Engineering Fracture Mechanics, vol. 73, no. 14, pp. 1959–1979, 2006. View at: Publisher Site  Google Scholar
 L. F. S. Parise, C. Ruggieri, and N. P. O'Dowd, “Fullyplastic strainbased J estimation scheme for circumferential surface cracks in pipes subjected to reeling,” Journal of Pressure Vessel Technology, vol. 137, no. 4, p. 041204, 2015. View at: Publisher Site  Google Scholar
 R. A. Ainsworth, “The assessment of defects in structures of strain hardening material,” Engineering Fracture Mechanics, vol. 19, no. 4, pp. 633–642, 1984. View at: Publisher Site  Google Scholar
 Y. J. Kim, J. S. Kim, Y. Z. Lee, and Y. J. Kim, “Nonlinear fracture mechanics analyses of part circumferential surface cracked pipes,” International Journal of Fracture, vol. 116, no. 4, pp. 347–375, 2002. View at: Publisher Site  Google Scholar
 Y. J. Kim and P. J. Budden, “Reference stress approximations for J and COD of circumferential throughwall cracked pipes,” International Journal of Fracture, vol. 116, no. 3, pp. 195–218, 2002. View at: Publisher Site  Google Scholar
 Y. J. Kim, J. S. Kim, Y. J. Park, and Y. J. Kim, “Elasticplastic fracture mechanics method for finite internal axial surface cracks in cylinders,” Engineering Fracture Mechanics, vol. 71, no. 78, pp. 925–944, 2004. View at: Publisher Site  Google Scholar
 N. H. Kim, C. S. Oh, Y. J. Kim, J. S. Kim, D. W. Jerng, and P. J. Budden, “Limit loads and fracture mechanics parameters for thickwalled pipes,” International Journal of Pressure Vessels and Piping, vol. 88, no. 10, pp. 403–414, 2011. View at: Publisher Site  Google Scholar
 D. H. Cho, H. B. Seo, Y. J. Kim, Y. S. Chang, M. J. Jhung, and Y. H. Choi, “Advances in Jintegral estimation of circumferentially surface cracked pipes,” Fatigue & Fracture of Engineering Materials & Structures, vol. 34, no. 9, pp. 667–681, 2011. View at: Publisher Site  Google Scholar
 J. S. Park, Y. H. Choi, and S. Im, “Generation of plastic influence functions for Jintegral and crack opening displacement of thinwalled pipes with a short circumferential throughwall crack,” International Journal of Pressure Vessels and Piping, vol. 117118, pp. 17–24, 2014. View at: Publisher Site  Google Scholar
 D. H. Cho, S. W. Woo, Y. S. Chang et al., “Enhancement of J estimation for typical nuclear pipes with a circumferential surface crack under tensile load,” Journal of Mechanical Science and Technology, vol. 24, no. 3, pp. 681–686, 2010. View at: Publisher Site  Google Scholar
 K. R. Jayadevan, E. Østby, and C. Thaulow, “Fracture response of pipelines subjected to large plastic deformation under tension,” International Journal of Pressure Vessels and Piping, vol. 81, no. 9, pp. 771–783, 2004. View at: Publisher Site  Google Scholar
 API 1104, Welding of Pipelines and Related Facilities, American Petroleum Institute, Washington, DC, USA, 2013.
 G. R. Irwin, “Plastic zone near a crack and fracture toughness,” Sagamore Research Conference Proceedings, vol. 4, pp. 63–78, 1961. View at: Google Scholar
 T. L. Anderson, Fracture Mechanics: Fundamentals and Applications, CRC Press, Boca Raton, FL, USA, 2005.
 A. A. Ilyushin, “The theory of small elasticplastic deformations,” Prikadnaia Matematica i Mekhanika, vol. 10, pp. 347–353, 1946, in Russian. View at: Google Scholar
 Y. J. Kim, D. J. Shim, K. Nikbin, Y. J. Kim, S. S. Hwang, and J. S. Kim, “Finite element based plastic limit loads for cylinders with partthrough surface cracks under combined loading,” International Journal of Pressure Vessels and Piping, vol. 80, no. 78, pp. 527–540, 2003. View at: Publisher Site  Google Scholar
 DNVRPF108, Fracture Control for Pipeline Installation Methods Introducing Cyclic Plastic Strain, Det Norske Veritas, Oslo, Norway, 2006.
 N. Nourpanah and F. Taheri, “Ductile crack growth and constraint in pipelines subject to combined loadings,” Engineering Fracture Mechanics, vol. 78, no. 9, pp. 2010–2028, 2011. View at: Publisher Site  Google Scholar
 N. Mostaghel and R. A. Byrd, “Inversion of RambergOsgood equation and description of hysteresis loops,” International Journal of NonLinear Mechanics, vol. 37, no. 8, pp. 1319–1335, 2002. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2018 X. Liu et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.